chapter 5 thermally activated processes and diffusion in solids 5-1

Post on 22-Dec-2015

227 views

Category:

Documents

Embed Size (px)

TRANSCRIPT

• Slide 1
• CHAPTER 5 Thermally Activated Processes and Diffusion in Solids 5-1
• Slide 2
• Copyright The McGraw-Hill Companies, Inc. Permission required for reproduction or display Rate Process in Solids Reactions occur in solid state resulting in more stable atomic arrangement. Reacting atoms must have sufficient energy to overcome activation energy barrier. At a given temperature, not all atoms have activation energy E*. It should be supplied to them. E r = Energy of reactants E* = Activation Energy Level E* = Activation Energy E p = Energy of Products Figure 5.1 5-2
• Slide 3
• Copyright The McGraw-Hill Companies, Inc. Permission required for reproduction or display Rate Process in Solids (Cont..) As temperature increases, more and more atoms acquire activation energy level. Probability of finding an atom/molecule with energy E* greater than average energy E of all atoms/ molecules is given by (After Boltzmann studied the effect of temperature on increasing the energies of gas molecules.) k = Boltzmanns Constant = 1.38 x 10 -23 J/(atom K) T = Temperature in Kelvin. 5-3
• Slide 4
• Copyright The McGraw-Hill Companies, Inc. Permission required for reproduction or display Rate Process in Solids (Cont..) The fraction of atoms having energies greater than E* in a system (when E* is greater than average energy E) is given by (Boltzmann equation) n = Number of molecules greater than energy E* N total = Total number of molecules k = Boltzmanns Constant= 8.62 x 10 -5 eV/K C = Constant T = Temperature in Kelvin. 5-4
• Slide 5
• Copyright The McGraw-Hill Companies, Inc. Permission required for reproduction or display Rate Process in Solids (Cont..) The number of vacancies at equilibrium at a particular temperature in a metallic crystal lattice is given by n v = Number of vacancies per m 3 of metal E v = Activation Energy to form a vacancy (eV) T = Absolute Temperature. k = Boltznam,s Constant = 8.62 x 10-5 eV/K C = Constant 5-5
• Slide 6
• Copyright The McGraw-Hill Companies, Inc. Permission required for reproduction or display Arrhenius Equation The rate of chemical reaction is given by Arrhenius equation. Rate of reaction = Ce -Q/RT Q = Activation energy J/mol or cal/mol R = Molar gas constant = 8.314 J/mol K or 1.987 cal/mol K T = Temperature in Kelvin C = Rate constant (Independent of temperature) Rate of reaction depends upon number of reacting molecules. 5-6
• Slide 7
• Copyright The McGraw-Hill Companies, Inc. Permission required for reproduction or display Solidification of Metals Arrhenius equation can also be written as ln (rate) = ln ( C) Q/RT or log 10 (rate) = log 10 (C) Q/2.303 RT Which is similar to Y = b + m X Which is equation of a straight line with Y intercept as b and slope m. Y log 10 (rate) X (1/T) b Log 10 (C) m Q/2.303R Figure 5.2Arrhenius plot (After J. Wulff et al., Structure and Properties of Materials, vol. II: Thermodynamics of Structure, Wiley, 1964, p.64.) 5-7
• Slide 8
• Copyright The McGraw-Hill Companies, Inc. Permission required for reproduction or display Atomic Diffusion in Solids Diffusion is a process by which a matter is transported through another matter. Examples: Movement of smoke particles in air : Very fast. Movement of dye in water : Relatively slow. Solid state reactions : Very restricted movement due to bonding. 5-8
• Slide 9
• Copyright The McGraw-Hill Companies, Inc. Permission required for reproduction or display Vacancy or Substitutional Diffusion Mechanism Atoms diffuse in solids if Vacancies or other crystal defects are present There is enough activation energy Atoms move into the vacancies present. More vacancies are created at higher temperature. Diffusion rate is higher at high temperatures. 5-9
• Slide 10
• Copyright The McGraw-Hill Companies, Inc. Permission required for reproduction or display Substitutional Diffusion Example: If atom A has sufficient activation energy, it moves into the vacancy self diffusion. As the melting point increases, activation energy also increases Activation Energy of Self diffusion Activation Energy to form a Vacancy Activation Energy to move a vacancy =+ 5-10
• Slide 11
• Copyright The McGraw-Hill Companies, Inc. Permission required for reproduction or display Interstitial Diffusion mechanism Atoms move from one interstitial site to another. The atoms that move must be much smaller than the matrix atom. Example: Carbon interstitially diffuses into BCC or FCC iron. Interstitial atoms Matrix atoms Figure 5.5 5-11
• Slide 12
• Copyright The McGraw-Hill Companies, Inc. Permission required for reproduction or display Steady State Diffusion There is no change in concentration of solute atoms at different planes in a system, over a period of time. No chemical reaction occurs. Only net flow of atoms. C1C1 C2C2 Net flow of atoms Per unit area per Unit time = J Solute atom flow Diffusing atoms Unit Area Concentration Of diffusing atoms Distance x Figure 5.6 5-12
• Slide 13
• Copyright The McGraw-Hill Companies, Inc. Permission required for reproduction or display Ficks First Law The flux or flow of atoms is given by I.e. for steady state diffusion condition, the net flow of atoms by atomic diffusion is equal to diffusivity D times the diffusion gradient dc/dx Example: Diffusivity of FCC iron at 500 o C is 5 x 10 -15 m 2 /s and at 1000 o C is 3 x 10 -11 m 2 /s J = Flux or net flow of atoms D = Diffusion coefficient = Concentration Gradient 5-13
• Slide 14
• Copyright The McGraw-Hill Companies, Inc. Permission required for reproduction or display Diffusivity Diffusivity depends upon Type of diffusion : Whether the diffusion is interstitial or substitutional. Temperature: As the temperature increases diffusivity increases. Type of crystal structure: BCC crystal has lower APF than FCC and hence has higher diffusivity. Type of crystal imperfection: More open structures (grain boundaries) increases diffusion. The concentration of diffusing species: Higher concentrations of diffusing solute atoms will affect diffusivity. 5-14
• Slide 15
• Copyright The McGraw-Hill Companies, Inc. Permission required for reproduction or display Non-Steady State Diffusion Concentration of solute atoms at any point in metal changes with time in this case. Ficks second law:- Rate of compositional change is equal to diffusivity times the rate of change of concentration gradient. Plane 1 Plane 2 Change of concentration of solute Atoms with change in time in different planes 5-15
• Slide 16
• Copyright The McGraw-Hill Companies, Inc. Permission required for reproduction or display Ficks Second Law Solution C s = Surface concentration of element in gas diffusing into the surface. C 0 = Initial uniform concentration of element in solid. C x = Concentration of element at distance x from surface at time t. x = distance from surface D = diffusivity of solute t = time. 5-16
• Slide 17
• Copyright The McGraw-Hill Companies, Inc. Permission required for reproduction or display Industrial Applications of Diffusion Case Hardening Sliding and rotating parts needs to have hard surfaces. These parts are usually machined with low carbon steel as they are easy to machine. Their surface is then hardened by carburizing. Steel parts are placed at elevated temperature (927 0 C) in an atmosphere of hydrocarbon gas (CH 4 ). Carbon diffuses into iron surface and fills interstitial space to make it harder. 5-17
• Slide 18
• Copyright The McGraw-Hill Companies, Inc. Permission required for reproduction or display Typical Gas-Carburized Steel Parts 5-18
• Slide 19
• Copyright The McGraw-Hill Companies, Inc. Permission required for reproduction or display Carburizing Low carbon Steel part Diffusing carbon atoms C % Figure 5.11 b Carbon Gradients In Carburized metals (After Metals handbook, vol.2: Heat Treating, 8 th ed, American Society of Metals, 1964, p.100) 5-19
• Slide 20
• Copyright The McGraw-Hill Companies, Inc. Permission required for reproduction or display Carburizing 5-20
• Slide 21
• Copyright The McGraw-Hill Companies, Inc. Permission required for reproduction or display Carburizing 5-21
• Slide 22
• Copyright The McGraw-Hill Companies, Inc. Permission required for reproduction or display Impurity Diffusion into Silicon Wafer Impurities are made to diffuse into silicon wafer to change its electrical characteristics. Used in integrated circuits. Silicon wafer is exposed to vapor of impurity at 1100 0 C in a quartz tube furnace. The concentration of impurity at any point depends on depth and time of exposure. Figure 5.12 (After W.R. Runyan, Silicon Semiconductor Technology, McGraw-Hill, 1965.) 5-22
• Slide 23
• Copyright The McGraw-Hill Companies, Inc. Permission required for reproduction or display Impurity Diffusion into Silicon Wafer (After W.R. Runyan, Silicon Semiconductor Technology, McGraw-Hill, 1965.) 5-23
• Slide 24
• Copyright The McGraw-Hill Companies, Inc. Permission required for reproduction or display Effect of Temperature on Diffusion Dependence of rate of diffusion on temperature is given by or D = Diffusivity m 2 /S D 0 = Proportionality constant m 2 /S Q = Activation energy of diffusing species J/mol R = Molar gas constant = 8.314 J/mol K T = Temperature (K) 5-24
• Slide 25

Recommended